Barium borate: Wikis

Note: Many of our articles have direct quotes from sources you can cite, within the Wikipedia article! This article doesn't yet, but we're working on it! See more info or our list of citable articles.

Encyclopedia

(Redirected to Beta barium borate article)

Beta barium borate (β-barium borate, BBO or β-BaB2O4) is a crystal frequently used for frequency mixing and other nonlinear optics applications. It has a wide transmission range, from approximately 200 nanometres to beyond 3 micrometres, and is used particularly for its transparency in the deep ultraviolet.

BBO has a trigonal crystal system, belongs to crystallographic point group 3m, and belongs to the crystallographic space group R3c. BBO has strong negative uniaxial birefringence and can be phase-matched for type I (ooe) second harmonic generation from 409.6–3500 nm. The temperature sensitivity of the indices of refraction is low, leading to an unusually large (55 °C) temperature phase-matching bandwidth. The crystal is mildly hygroscopic.

β-Barium borate differs from α-barium borate in the positions of the barium ions within the crystal. Both phases are birefringent, however the α phase, which exists above 925 °C, possesses centric symmetry and thus does not have the same nonlinear properties as the β phase.[1]

BBO is a common material used to split photons to produce the phenomenon of quantum entanglement.

Physical properties

• Lattice parameters: a=b=1.253 nm, c=1.272 nm, Z=6
• Melting point: 1095±5 °C
• Phase transition temperature: 925±5 °C
• Mohs hardness: 4.5
• Density: 3.85 g/cm3

Optical properties

• Refractive index, 1064 nm: $n_o=1.65, \quad n_e=1.54$
• Refractive index, 532 nm: $n_o=1.67, \quad n_e=1.55$
• Refractive index, 266 nm: $n_o=1.75, \quad n_e=1.61$
• Transparency range (> 0.5 cm-1): 198–2600 nm[1]
• Thermo-optic coefficients:[1]
• $\frac{\partial n_o}{\partial T}= -9.3 \times 10^{-6} / \mathrm{^\circ C}$
• $\frac{\partial n_e}{\partial T} = -16.6 \times 10^{-6} / \mathrm{^\circ C}$
• Nonlinear optical coefficients: [2]
d22 = 2.3 pV / m.
d31 = -0.16 pV / m.
• High damage threshold of 10 GW/cm2 for 100 ps pulse-width at 1064 nm.

Sellmeier equations (for λ in micrometres)

• $n^2_o(\lambda)$ = 2.7359+0.01878/(λ2 - 0.01822)-0.01354 λ2 [3]
• $n^2_e(\lambda)$ = 2.3753+0.01224/(λ2-0.01667)-0.01516 λ2 [3]

References

1. ^ a b c D. N. Nikogosyan. "Beta Barium Borate (BBO)". Applied Physics A 52: 359--368.
2. ^ V.G. Dmitriev, G. G. Gurzadyan, and D. N. Nikogosyan (1999). Handbook of Nonlinear Optical Crystals, 3rd edition. Springer. ISBN 0342-4111.
3. ^ a b Kato, K. (1986). "Second-harmonic generation to 2048 Å in β-BaB2O4". IEEE Journal of Quantum Electronics 22 (7): 1013--1014. doi:10.1109/JQE.1986.1073097.